Definition of fresh concrete:
The potential strength and durability of concrete of a given mix proportion
is very dependent on the degree of its compaction. It is vital, therefore,
that the consistency of the mix be such that the concrete can be
transported, placed, and finished sufficiently early enough to attain the
expected strength and durability.
Properties of Fresh Concrete:
The first 48 hours are very important for the performance of the concrete
It controls the long-term behavior, influence f'c (ultimate strength), Ec
(elastic modulus), creep, and durability.
Elasticity and Strength of Concrete:
The elastic properties of materials are a measure of their resistance to
deformation under an applied load (but the elastic strain is recovered when
the load is removed).
Strength usually refers to the maximum stress that a given kind of
sample can carry.
Understanding these properties and how they are measured is essential
for anyone wishing to use materials.
Properties of Fresh Concrete :
Properties at Early Ages :
Time of Set
Properties of Fresh Concrete:
Definition: Effort required to manipulate a concrete mixture with a minimum
It is not a fundamental property of concrete.
I) consistency (slump) how easy to flow
II) cohesivenesstendency to bleed and segregate
Themost important properties of fresh concrete are thus associated with
its workability and consistency.
Most concrete must be compacted after it has been placed in theforms.
Whether the compaction is achieved by raming or by vibration, the
process consists essentially of the eliminationof entrapped airfrom the
it has achieved as dense a configuration as possible for a given mix.
Large pockets of entrapped air seriouslyweaken the concrete since they
This term is defined in ASTM C 125 as the property determining the
effort required to manipulate a freshly mixed quantity of concrete with
minimum loss of homogeneity.
The term manipulate includes the operations of placing, compacting and
finishing the concrete.
Neville and Brooks* define workability as the amount of useful
They note that the useful internal work is a physical property internal
work necessary to produce full compaction. of the concrete alone, but they
note there is additional energy
required to overcome friction between the concrete and the formwork and
the reinforcement as well as the energy required to vibrate the formwork,
the reinforcement, and the concrete which has already been compacted.
Thus in practice, it is difficult to measure the workability as defined.
Stiffening and Setting:
After completion of mixing, concrete gradually stiffens until it becomes
It is essential that it remain plastic long enough to permit being
transported, placed, consolidated, and finished.
Initial Set: Loss of consistency, unworkable concrete (no less than
45 minutes – ASTM C 150)
Final Set: Complete solidification (no more than 375 minutes)
Compacting Factor Tests:
Although there is no generally accepted method of directly measuring
workability, Neville and Brooks* point out that probably the best test yet
available uses the inverse
approach: i.e., the degree of compaction can be measured when a
standard amount of work is applied to a standard quantity of concrete.
Thedegree of compaction, called the compacting factor, is measured
by the density ration which is the ratio of the density actually achieved in
the test to the density of the same concrete fully compacted.
These tests are covered in the United States underACI 211.3, and in the
UK by BS 1881: Part 103: 1983.
The Kelly Ball Test:
Another method used in the field and laboratory to measure the
consistency of concrete is the ball penetration test (ASTM C360) which is
also known as the Kelly ball test.
It is performed by measuring the penetration, in inches, of a 6-in.
diameter steel cylinder with a hemispherically shaped bottom, weighing 30
One of the advantages of the ball penetration test can beperformed on
the concrete in a hopper, buggy, wheelbarrow, or other suitable container.
Another advantage of this method is its simplicity and the rapidity with
which the consistency of the concrete can be determined.
It is also not dependent on a procedure of filling and rodding acontainer
like the slump test.
The most common method of measuring the air content of freshly mixed
concrete is the “pressure method” (ASTM C231).
Inthis method, pressure is applied to a concrete sample placed into an
air meter and the reduction in volume observed on
a gage calibrated in terms of percent air.
The observed amount of air includes both the purposely entrained air as
well as the entrapped air (about 1% by volume of concrete).
Don’t Use More Water!:
What is sometimes regarded as a need for wetter concrete may be better
satisfied by more thorough vibration.
The use of adequate vibration rather than of a wetter mix will not only
insure a more thorough compaction but also the quality of concrete will be
superior by not increasing the
water content to obtain a greater slump.
The Careful attention to keeping the mix as dry as possible and being
sure that there is adequate vibration will lead to sound concrete.
The worst combination; however, is to “over” vibrate concrete which is
Consistency or fluidity of concrete is an important component of
workability and refers in a way to the wetness of the concrete.
However, it must not be assumed that the wetter the mix the more
workable it is. If a mix is too wet, segregation may occur with resulting
honeycomb, excessive bleeding,
and sand streaking on the formed surfaces.
On the other hand, if a mix is too dry it may be difficult to place and
compact, and segregation may occur because of lack of
cohesiveness and plasticity of the paste.
Workability and Consistency:
In their textbook, Mehta and Monteironote that workability is a composite
property, with at least two main
a. Consistency which he describes as the “ease of flow” of the concrete,
b. Cohesiveness which he describes as the “tendency not to bleed or
Someof the important factors that affect the
workability of concrete are:
1) relative quantities of paste and aggregates,
2) plasticity of the paste itself,
3) maximum size and grading of aggregates, and
4) shape and surface characteristics of aggregate
Each of these factors effectthe components of workability, consistency
and cohesiveness, in different ways.
Mehta and Polivka* discuss further that:
None of the test methods proposed or in use today simultaneously
measure all of the properties involved in workability.
In practice, the workability of a mix is judged by several properties
including consistency, ease of conveying and placing, and lack of
segregation or of excessive bleeding.
An experienced concrete technician can readily judge when fresh
concrete has adequate workability for use in a given situation.
A concrete mix suitable for massive construction, e.g., of a bridge pier,
would not have the required workability for
placement in a heavily reinforced column.
Thus, a concretemix should have the needed workability for its intended
use. Also, it should not segregate nor bleed excessively.
Workability and consistency of fresh concrete are two closely related
properties. Workability is that property of freshly mixed concrete which
determines the ease and homogeneity with which it can be mixed,
transported, placed, compacted, and finished.